Denunciar

IRJET JournalSeguir

12 de Apr de 2023•0 recomendaciones•2 vistas

12 de Apr de 2023•0 recomendaciones•2 vistas

Denunciar

Ingeniería

https://www.irjet.net/archives/V10/i2/IRJET-V10I2101.pdf

IRJET- EBR and GM Methods for External Flexural Strengthening of RC BeamsIRJET Journal

IRJET- Flexural Strengthening of Pre-Cracked Corroded RC Beams using CFRP SheetsIRJET Journal

Behavior of RC Beams Retrofitted/Strengthened With External Post-Tension SystemINFOGAIN PUBLICATION

IRJET- Numerical Analysis of RC Beams Reinforced with CFRP RodsIRJET Journal

IRJET- Investigation on EBROB Method to Postpone Debonding of CFRP Sheet Comp...IRJET Journal

Experimental investigation of the crashworthiness performance of laminated co...IRJET Journal

- 1. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 685 Investigating the Effect of Prestressing CFRP Laminate and Mechanical Anchorage to Strengthen Steel Beams Under Flexural Loading Mohamed A. Gharib 1, Ali El Awadi 2 1 alfanar Engineering Services, mo.g.abdul.76@gmail.com 2 Teaching and Research Assistant, Zagazig University, Zagazig, Egypt, cengag2@gmail.com ---------------------------------------------------------------------***--------------------------------------------------------------------- Abstract - The use of composite materials, such as Carbon Fiber Reinforced Polymer (CFRP), as a strengthening and retrofitting method for steel beams, has gained widespread attention in recent years. This study aims to improve the understanding of the behavior of steel beams reinforced with CFRP laminates with mechanical anchorage. The previous analytical studies did not include the effect of mechanical anchorage. This study examines the behavior of steel I-beams strengthened withprestressedcarbonfiberreinforcedpolymer (CFRP) laminate and fixed with mechanical anchorage under flexural loading. An experimental program, a closed-form analytical model, and a finite element analysis are presented in this investigation. Ten steel beams were experimentally investigated with and without mechanical anchorage and at various prestressing levels. An analytical and a finite element model considering the mechanical anchorage were developed to predict the stresses in the CFRP-Steel beam adhesive layer at the contact area. The models were validated with experimental results. The mechanical anchorage successfully increased the bond strength and changed the failure mode from premature debonding to CFRP rupture. The study highlights the importance of considering mechanical anchorage in analytical models for bonded CFRP laminates to ensure the preservation of prestressing force. Key Words: CFRP, Mechanical Anchorage, Prestressing, Cohesive Zone Methos, Crack Propagation. 1. INTRODUCTION The use of CFRP laminate in retrofitting substandard steel beams is not popular as its use for retrofitting concrete structures [1 & 5]. The strengthening process includes the adhesion of a CFRP layer to the steel beam lower flange [2 & 3]. This configuration has a major problem which is the debonding failure of between the steel beam and the CFRP strip. It was found from previous studies that prestressing the CFRP layer may improve the performance utilize the full capacity of the strengthened hybrid beam. Previous investigations found that prestressing the CFRP laminates is beneficial to the strengthening process [4]. Several techniques are suggested to apply the pretension force to the CFRP laminate in such a configuration. Mechanical anchorage is required for the effectiveness of these techniques. The proposed mechanical anchorage is applied at both ends of the laminate. This can result in an enhanced ductile behaviour and increase the prestressing force that can be applied. Using mechanical anchorage improves the serviceability and strength of the composite sections [2 & 6]. Previous studies that employed the finite element method to investigate the behaviour of this strengthening technique used the smeared crack concept to analyse the interfacial stress resulting from thecontactzone between the steel beam and the CFRP laminates [7]. On the other hand, the discrete damage method reﬂects the ﬁnal damaged condition more accurately. It models the crack propagation through a displacement–discontinuityusing an interface element that separates two sides of the crack modelled using solid elements such as the cohesive zone method (CZM). This method presupposes that the stress between two surfaces of two materials does not dissipate immediately when damage is initiated at their interface. The cohesive material behaviour controls the interface between the separating surfaces of the steel beam and the laminate. The CZM act as a spring between the element connectingthe modelled surfaces. However, the stiffness of the element is part of the structural stiffness, so the element deformation will occur during the loading of the laminate. Analytical models in previous studies were introduced to calculate the shear and normal stress in the contact zone between the steel surface and the CFRP layer attached to it [8, 9 &10]. However, these studies did not considerthesignificanteffect of mechanical anchorage if employed. This study utilized an experimental programtoevaluate and analyze the behavior of steel beams reinforced with prestressed CFRP using mechanical anchorage under flexural loading at two points. A total of ten steel beams reinforced with various configurations of prestressed CFRP laminates were subjected to static flexural loading until failure occurred. The specimens were simulated using the CZM approach and finite element method. The accuracy of the FE model was validated by comparing it with the results obtained from the experimental program. TheFEmodel was then utilized to evaluate the impact of increased prestressing. Furthermore, an analytical investigation was introduced to predict the interfacial shear and normal stresses on the adhesive layer of the examined beams. The analytical model's findings were compared against both the FEM and experimental program results. Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 2. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 686 2. THE EXPERIMENTAL PROGRAM The experimental program considered several key factors, including the prestressing levels, yield strength of the steel beam, and mechanical anchorage implemented at both ends of the CFRP laminate. The jacking system setup shown in Figures (1) and (2) is used to apply the load to the strengthened beams. Fig -1: Test Setup Fig -2: Test sample preparation and applying the pre- stressing force / prestressing tool detail 2.1 Description of the Beams The experimental program's test specimen details are presented in Table (1). The first specimen has a section size of IPE160, while the other nine beams haveacross-sectionof W 6x20, with a steel beam length of 2.9 m. SpecimenCB2was reinforced with bonded CFRP and was not prestressed. The CFRP laminate thickness used for all specimens was 1.2 mm. Table -1: Test Specimen Details Specimen CFRP laminate Anchorage Pretension Force (KN) TB 50 Yes NA CB1 No No NA CB1A No No NA CB2 100 No NA B1-25-NA 100 No 25 B2-45-NA 100 No 45 B3-25-AN 100 Yes 25 B4-45-AN 100 Yes 45 B5-25-AN 50 Yes 25 The CFRP laminate used to reinforce the specimens is 100 mm wide, with the exception of TB and B5-25-AN, which have a 50 mm wide CFRP strip. The thickness of the CFRP laminates for all specimens is 1.2 mm. Specimen B6-45-AN- NAD features a 100 mm pre-stressed CFRP laminate and mechanical end anchorage, but no adhesive layer was applied between the steel beam's lower flange and the CFRP laminate. Figure (3) illustrates the beam's cross-section and the CFRP layer. Fig -3: Cross section of the steel beam, adhesive, CFRP strip and the grip plates 2.2 Material Properties The mechanical properties of the steel beam and the CFRP strips were determined through standard testing and from the manufacturer's datasheet. The average yield strength of the steel beam material is 390 MPa, and its ultimate tensile strength was measured to be 560 MPa. The CFRP strips used in this investigation consist of pitch- based carbon fibers and epoxy resin, with thicknesses of 1.2 mm and widths of 50 mm or 100 mm. The fiber volume fraction of the strips is 68%. The CFRP laminate has an average ultimate strength of 3,100 MPa and an average measured elasticity modulus of 165 GPa [27]. A two-component epoxy adhesive was utilized to bond the CFRP laminate to the steel beam's surface. The adhesive's mechanical properties, as provided by the manufacturer's datasheet [28], are listed in Table (2). Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 3. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 687 Table -2: Properties of the epoxy material Mechanic al propertie s Tensile strengt h Compressiv e strength Shear strengt h Bond strengt h Tensile modulus Value (MPa) 24.8 61 24.8 18 4,400 2.3 Test Set-up Figure (1) depicts the experimental setup used in this study, which consists of simply supported beams subjectedtotwo- point loads. The load was applied to the beam using a universal testing machine. To measure the deflection, a displacement transducer was installed at mid-span. Additionally, strain gauges were mounted on the CFRP laminate and at the mid-span of thebeamflangestomeasure strain. 2.4 Experimental results 2.4.1 Failure Modes In this study, applying prestressing to the CFRP laminate resulted in a proportional decreaseindeflectionanddelayed premature debonding failure. The control beams CB-1 and CB-1A failed in a typical flexural manner. On the other hand, beam CB-2, strengthened with non-prestressed CFRP laminate, experienced a 1.2% increaseinthefailureload due to laminate debonding. CFRP-prestressed beamsB1-25-NAandB2-45-NAfaileddue to debonding of the CFRP laminate from the steel bottom flange immediately after releasing the grip anchor at both ends of the beam. However, CFRP-prestressedbeamsB3-25- AN and B5-25-AN with end anchorage and Fy = 390 MPa failed in a typical flexural manner, with the CFRP laminate experiencing a sudden rupture failure and a significant increase in the failure load compared to the non- strengthened control beam CB-1. These beams developed a full plastic hinge at failure without encountering premature debonding. The same failure mode was observed for beam B4-45-AN, but with a lower achieved strength enhancement of 3.3% in yield load. The behavior of beam B6-45-AN-NAD, which had end anchorage but no adhesive, was similartothatofbeams with end anchorage and adhesive in terms of flexural behavior, but the increase in failure load was less than for specimens strengthened using the adhesive layer, at 7% compared to the original non-strengthened beam CB-1. The CFRP laminate in this beam ruptured at a load of 186 kN, earlier than in the corresponding specimenwithendanchorage and adhesive layer. Table 3 provides a summary of the results obtainedfromthe experimental investigation. Fig -4: Typical CFRP rupture in tested beams Table-3a: Results of the experimental investigation - Yield Load Beam No. CFRP Jacking Strain ( ) Yield Load Py (kN) Py / PyCB% TB 3050 108.1 - CB1 – 172.7 - CB1A – 161.0 - CB2 – 174.8 - B1-25-NA 3092 N/A - B2-45-NA 4021 N/A - B3-25-AN 3140 193.0 12% B4-45-AN 3984 166.3 3% B5-25-AN 3103 195.2 13% B6-45-AN- NAD 4011 184.3 6.5% Table-3b: Results of the experimental investigation – Debonding Load Beam No. CFRP debonding load CFRP Failure Pde (kN) Associated Strain ( ) TB No debonding No debonding No Failure CB1 N/A N/A N/A CB1A N/A N/A N/A CB2 193.2 5290 Debonding Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 4. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 688 B1-25-NA 64.8 15.16 Debonding B2-45-NA 76.33 16.48 Debonding B3-25-AN 204.5 3953 Rupture B4-45-AN 178.9 5725 Rupture Table-3c: Results of the experimental investigation- Rupture Load Beam No. CFRP rupture load CFRP Failure Pfru (kN) Associated Strain ( ) B3-25-AN 199.7 4435 Rupture B4-45-AN 190.5 9601 Rupture B5-25-AN 202.3 12101 Rupture B6-45-AN-NAD 186.0 857 Rupture 2.4.2 Load-displacement relationship The specimen TB failed due to lateral torsional buckling, but no debonding or CFRP rupture was observedduringthetest. The predicted yield load of the specimen was Py=93.3 kN. However, based on experimental results,themeasuredyield load was 108.16 kN at a corresponding deflection of 22.44 mm. This indicates a 16% increase in the yield load capacity of the strengthened section when comparedtothepredicted yield load. The load deflection response of specimen B5-25-AN was compared to that of the control beam CB1. During the test, there was no debonding or CFRP ruptureobservedinB5-25- AN. The yield load of CB1 was 172.7 kN at a corresponding deflection of 20.46 mm, whereas the yield load of B5-25-AN was 195.2 kN at a corresponding deflection of 26.28 mm, indicating a 13% increase in the yield load capacity of the combined strengthened section. The final failure load of B5- 25-AN was 200.7 kN at a corresponding deflection of 93.45 mm, while the final failure load of CB1 was 187 kN at a corresponding deflection of 82.63 mm. Specimen CB2 attained its yield capacity without any observed premature failure. The yield load of specimen CB2 was measured to be 174.8 kN at a corresponding deflection of 19.5 mm, indicating that the CFRP strengthening, with neither prestressing nor mechanical anchorage, only increased the yield strength of the combined section by 1.2%. However, the specimen experienced a debonding failure and a sudden drop in the applied load after further loading. The debonding load for specimen CB2 was measured to be 193.2 kN at a corresponding deflection of 29.33 mm. After debonding, the specimen was un- strengthened and behaved similarly to control beam CB1 until final failure. The load deflection response of specimen B3-25-AN was compared to that of the control beams CB1 and CB2. The yield load for specimen B3-25-AN was measured to be 194.66 kN at a corresponding deflection of 21.07 mm, indicating a 13% increase in the yield load capacity of the combined strengthened section compared to control beam CB1. During the plastic stage, the specimen experienced a load drop, combined with a sudden deflection at mid-span caused by CFRP rupture at a load of 199.7 kN and a corresponding deflection of 37.05 mm. The specimen exhibited a second and final rupture at a load of 197.8 kN at a corresponding deflection of 57.53 mm before the section became un-strengthened and had the same behaviorasboth control beams until final failure. The load deflection response for specimen B4-45-AN was compared to that of control beam CB1A. Both specimens reached their yield capacity without any premature failure observed. The measured yield load for specimen CB1A was 161 kN at a corresponding deflection of 22 mm, while the measured yield load for specimenB4-45-AN was166.3kN at a corresponding deflection of 23.34 mm. This indicates only a 3.3% increase in the yield load capacity. Both specimens, B6-45-AN-NAD and CB1, exhibited similar load deflection responses. The specimens failed in a typical flexural manner, with no premature failure observed. The measured yield load for the specimen was attained with no significant difference compared to the control beam. Specimen B6-45-AN-NAD showed only a 7% increase in yield load capacity compared tothecontrol beamCB1,witha measured yield load of 184.3 kN at a corresponding deflection of 24.71 mm. Which shows how is the effect ofthe lack of the adhesive layer on the response and the overall strength. However, after further loading, the specimen experienced a rupture failure with a sudden drop in the applied load. The measured rupture loadforthisspecimenis 201.33 kN at a corresponding deflection of 39.67 mm. The specimen also exhibited a second and final rupture at a load of 202.33 kN at a corresponding deflection of 55.14 mm before the section became un-strengthened and behaved similarly to the control beam until final failure. Figure (5) shows the effect of adding CFRP strengthening and the advantage of prestressing the CFRP laminate which enhanced the overall performance of the beam. Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 5. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 689 Fig-5: Load–displacement relationship for un- strengthened beam vs CFRP strengthened beam with and without prestressing 3 FINITE ELEMENT ANALYSIS 3.1 Finite element model The ﬁnite element program ANSYS® (version 13) was used in this investigation[17].Athree-dimensionelement(3D FE) model was developed to simulate the geometric and nonlinear material behavioroftheinvestigated beams.Four- node shell element, (Shell 281), was used to model the steel beam. Eight-node brick element (Solid 185) was used to model the adhesive layer and the CFRP strip [11]. The area between the CFRP laminate and the steel beam was simulated using a 3-D 8-node linear interface element(Inter 205). This element, when used with the (Solid185) element, simulated the interface between two surfaces and the subsequent separation process, where the separation was represented by a gradual displacement between nodes representing the two bonded surfaces. 3.2 Boundary conditions Beams are symmetric about their longitudinal axis, and therefore only half of the beams were modeled. The beams were modeled with a roller support at one end and a hinged support at the other end. Two stiffening plates were welded to the steel beam's flange at the point of loading and at the supports to prevent stress concentration. The load was applied incrementally as a static load, following the automatic loadcontrol scheme.Themodifiedstandard/static general method was used for the analysis. Figure (6) depicts the simulated beam with applied forces and boundary conditions. Fig -6: Simulated beam with boundary conditions 3.3 Materials modeling In this study, the classical elastic-plastic material model with strain hardening was used to represent the steel I-beam, which has a bilinear stress-strain relationship for both compression and tension. The CFRP strip, on theotherhand, has a linear stress-strain relationship until failure. When brittle materials undergo tensile fracture, microcracking, tortuous debonding, and other internal damage processes occur progressively and eventually leadtotheformation ofa geometrical discontinuity that separates the material. If this discontinuity occurs within the same material, it is called a crack, while if it occurs between two different materials, itis referred to as debonding or delamination. In this research, the cohesive zone modelling approach (CZM) is used to simulate debonding. To implement this approach, a CZ material was created and assignedtothecontactelementsin the interface zone, and its behavior is described interms ofa traction-separation equation instead of the traditional engineering stress-strain (σ − ε) equation. To ensure the zero thickness of the element, coincident opposite nodes of the cohesive element are defined. The CZ material was characterized by three constants: the material's maximum allowed stress, the energy release rate at normal separation, and the tangential displacement at maximum stress. 3.4 Prestressing Effect There are many methods that can be used to simulate the prestressing effects on the CFRP laminates. In this investigation the constant prestressing effectinthelaminate was applied in the longitudinal (x) direction to the specific material of the CFRP using the software package. 3.5 The Simulated Beams The present study was conducted in two stages. Stage one focused on validating the present finite element analysis by analyzing numerically the steel beams that were previously tested in the experimental program. Five beams were Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 6. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 690 simulated at this stage to validate the finite element model. These included: 1. CB1: Control beam with no CFRP strengthening, having a steel yield strength of 390 MPa. 2. CB1A: Control beam with no CFRP strengthening, having a steel yield strength of 350 MPa. 3. CB2: Control beam with only one CFRP strengthening strip, 100mm wide, and a yield strength of 390 MPa. This beam was not subjected to any prestressing force. The CFRP strip was attached to the steel beam with a 1 mm layer of adhesive, without the use of mechanical anchorage. 4. B3: Beam strengthened with a 100 mm CFRP strip. The CFRP strip was subjected to 25 kN prestressing force. The yield strength of the steel beam was 390 MPa, and the CFRP laminate was attached to the steel beam using a 1 mm layer of adhesive material and two sets of mechanical anchorage, one at each end of the CFRP laminate. 5. B4: Beam similar in configuration to B3, but with a prestressing force of 45 kN and a yield strength of 350 MPa. In the second stage of the study, the FEM model was extended to investigate the effect of increasing the prestressing level on the behaviorofthe beam.Thevalidated FEM of the simulated beams from stage I was modified to evaluate the impact of increasing the prestressing force applied to the CFRP laminate. The beams tested at this stage were: 1. B3-15%: This beam has the same configuration as beam B3 introduced in stage I. However, the prestressing force applied to this beam was 15% of the ultimate tensile strength of the CFRP strip. 2. B3-40%: The prestressing force applied to this beam was 40% of the ultimate tensile strength of the CFRP strip. 3. B3-70%: The prestressing force applied to this beam was 70% of the ultimate tensile strength of the CFRP strip. 4. Figure (7) illustrates the load-displacement relationship for the simulated beam and the experimentally tested B4. Fig -7: Load–displacement relationship for simulated beam and experimentally tested CB2 4 PROPOSED ANALYTICAL MODEL AND THEORETICAL APPROACH The debonding failure mode is caused by interfacial stress concentration in the contact surface in the end zone. Closed- form solutions of such stresses are thus essential in developing any design guidelines for strengthening beams with bonded prestressing CFRP laminates. Consider a steel beam with a typical I – section strengthened with a prestressed laminate bonded to the tension side. Fig -8: Schematic sketch of analyzed beam For Simplification of the equations, the following assumptions were made: - It is assumed that all materials exhibit linear elastic behavior. - The stiffness of the steel beam is significantly greater than that of the CFRP laminate. - The principle of the plane section remaining plane after deformation is upheld. Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 7. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 691 - Bending deformations of the adhesive layer can be disregarded. - No slipping will occur at the interface area before failure. - The thin adhesive layer thickness maintains constant stresses. Figure (8) shows a schematic sketch of the beam strengthened with a bonded prestressed laminate where Pl is the residual prestressing force in the laminate. The loss of prestressing force in the laminates is: (1) However, in the case of using mechanical anchorage and applying adhesive layer, the loss of the prestressing Pl force can be neglected, and it can be assumed that Pl = P0, hence the prestressing force in the steel beam Ps can be expressed as below: (2) Analyzing a differential segment of a plated beam, where the interfacial shear and normal stresses are denoted by τ(x) and σ(x), respectively [26], the interfacial shear stress can be calculated as per below equations: 1st Interval: for , at this interval, the general solution for the interfacial shear stress considering value of Vs = P , is (3) 2nd Interval: for , at this interval, the general solution for the interfacial shear stress (4) The solution for the above equation is: (5) and (6) Where: (7) (8) (9) and (10) (11) And the adhesive normal stress can be expressed using below equations: 1st Interval: When , (12) 2nd Interval: , (13) Where: (14) (15) 5 RESULTS AND DISCUSSIONS 5.1 Analytical and numerical results Tables (4) and (5) present the analytical and numerical results of the investigated beams. The results show that strengthening the beam with non-prestressed CFRP and without mechanical anchorage only increased the yield load Py of the beam by 1.2%. However, when prestressing and mechanical anchorage were used, the yield load increased from 1.2% to 11.7%. Additionally, when the pretension load Pl was increased from 7% to 12%, the calculated adhesive shear stress at debonding load at peak τx=0 is reduced by 37%, and the calculated normal stress at debonding load at peak σx=0 was decreased by 30%. The FEM adhesive shear stress at debonding load at peak τx=0 is also decreased by 37%, and the FEM normal stress at debonding load at peak σx=0 was Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 8. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 692 decreased by 30% when the pretension load Pl is increased from 7% to 12%. Table-4: Calculated interfacial Stress for the specimens tested in the experimental program Sample TB B3-25 B4-45 B5-25 Prestressing Force P0 (kN) 25 25 45 25 Premature Failure Load (kN) 108 199.7 178.9 202.3 Failure Mode Torsional Buckling CFRP Rupture CFRP Rupture CFRP Rupture Calculated Peak Shear Stress (MPa) 34.4 31.5 28.7 32.8 Calculated Peak Normal Stress (MPa) 2.13 1.96 1.8 2.04 5.2 Calculated shear and normal stress on the adhesive layer at peak (laminates ends) Figure (9) displays the shear and normal stress distribution at a loading value of 100 kN for the investigated beams TB, B3, B4, and B5 when strengthened without mechanical anchorage at both ends of laminates. In contrast, Figure (10) shows the same analysis for the beams after considering the mechanical anchorage in the analysis with the newly developed equations. The analysis reveals that the mechanical anchorage neutralizes the effect of the mechanical properties of the adhesivelayer and the prestressinglevel.Thestressaffecting the adhesive layer at both ends of the CFRP laminates is controlled only by the mechanical properties of the steel beam. These findings are consistentwiththeresultsobtained from the experimentally tested beam B6-45-AN-NAD. Table-5: Experimental, Analytical and Numerical Results comparison Beam No. CB1 CB1A CB2 B3 B4 Experimental Yield Load PEy (kN) 172.7 161 174.8 193 166.3 Numerical Yield Load PFy (kN) 172.8 158.4 174.4 193.6 164.8 Experimental CFRP debonding load PEde (kN) N/A N/A 193.2 204.5 178.9 Experimental CFRP rupture load PEru (kN) N/A N/A No Rup. 199.7 190.5 Numerical CFRP debonding load PFde (kN) N/A N/A 193.6 212 187.2 Calculated Adhesive shear stress at debonding load at peak τx=0 N/A N/A N/A 31.5 28.7 Calculated Adhesive Normal stress at debonding load at peak σ x=0 N/A N/A N/A 1.96 1.8 FEM Adhesive shear stress at debonding load at peak τx=0 N/A N/A 0.13 7.94 3.61 FEM Adhesive Normal stress at debonding load at peak σ x=0 N/A N/A 0.94 2.38 1.93 (a) Shear stress (MPa) (b) Normal stress (MPa) Fig. -9. Adhesive interfacial Stress at Fixed Load P=100 kN and variable Distance from Laminate End without mechanical anchorage. Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 9. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 693 (a) Shear stress (MPa) (b) Normal stress (MPa) Fig. - 10. Adhesive interfacial Stress at Fixed Load P=100 kN and variable Distance from Laminate End with mechanical anchorage 5.3 Effect of pretension force level To investigate the effect of the pretension force level on the peeling load, threebeamswerenumericallystudied:B3-15%, B3-40%, and B3-70%, with prestressing forces Pl of 55.8 kN (15% of the CFRP laminate ultimate tensile load), 140.8 kN (40% of ultimate tensile load), and 260.4 kN (70% of the ultimate tensile load of the CFRP laminate), respectively. These beams were compared with the original beam B3, which had a prestressing force Pl of 25 kN (almost 7% of laminate ultimate tensile load). A comparison between the present finite element analysis (FEA) and the experimental results is shown in Table 6, which presents the yieldloadand ultimate load for each specimen. The results indicate that the applied loads versus mid-span deflections for the beams with different prestressing levels obtained from the FEA were almost similar. However, increasing the prestressing load Pl increases the yield load Py and the overall composite section stiffness while decreasing the ultimate load capacity. Increasing the prestressing load up to 70% enhanced the section performance, but the failure modechanged from debondingtoCFRPrupture.Therefore,it is recommended not to increase the prestressing level more than 40% of the laminate tensile capacity. Table-6: B3 FEA Failure Loads Beam No. Yield Load Py (kN) Ultimate Failure Load PU (kN) Mode of Failure PU / PU7% B3-7% 193.6 216 CFRP Debonding 1 B3- 15% 196.8 219.2 CFRP Debonding 1.014 B3- 40% 200 240 CFRP Debonding 1.11 B3- 70% N/A 135.2 CFRP Rupture 0.60 Previous studies have shownthatincreasingtheprestressing force from 7% to 40% results in a significant decrease in normal stress along the length of the CFRP strip at a concentrated load of P=100 kN, with the stress peak point located at the mechanical anchorage at the ends of the laminate, which is consistent with the prediction of the developed analytical model [26]. Using the analytical model and assuming a prestressing force of 40%, the effect of increasing the adhesive layer thickness and the CFRP width was analyzed. The results indicate that increasing the adhesive layer thickness has no significant effect on the shear stress at the peak point (x=a). However, increasing the adhesive layer thickness from 1mm to 2.5mm reduces the normal stress by 48%. Similarly, increasing the CFRP layer width from 5cm to 15cm reduces the calculated normal stresses by 3% at the peak load point when using a prestressing force of 45% at a 100kN point load. Table - 7 provides detailed results from the analytical model. Table-7 (a): Effect of increasing the adhesive layer thickness on the interfacial normal stress (at 100 kN load and 45% prestressing) Adhesive thickness Calculated normal stress at peak σ x=a (MPa) Ratio 1mm 1.808 1 1.5mm 1.340 26% 2mm 1.084 40% 2.5mm 0.932 48% Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 10. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 694 Table-7 (b): Effect of increasing the CFRP laminate width on the interfacial normal stress (at 100 kN load and 45% prestressing). CFRP laminate width Calculated normal stress at peak σ x=a (MPa) Ratio 5cm 1.834 0% 10cm 1.808 1% 12cm 1.798 2% 15cm 1.783 3% 3. CONCLUSIONS In conclusion, the experimental and analytical studies carried out in this research providevaluableinsightsinto the behavior of steel beams strengthened with CFRP laminates. It was found that the use of CFRP prestressing significantly increased the ultimate load capacity of the strengthened beam and delayed the premature debonding failure of the laminate. On the other hand, non-prestressedCFRPlaminate mainly failed due to premature debonding, withonlya slight increase in the failure load. The use of mechanical end anchorage was found to be essential inmaintainingtheCFRP laminate prestress after releasing the jacking force, while epoxy mortar alone was not sufficient for this purpose. It was also observed that increasing the CFRP prestressing level up to 12-15% of the laminate tensile capacity, even without using a mechanical anchorage, provided significant enhancement in the ultimate load capacity of the beam and prevented premature debonding failure. The adhesive properties did not affect the ultimate load, but they may influence delaying the debonding of the laminates, which is highly dependent on the efficiency of the anchorage system and the level of prestressing. Thicker clamp plates were recommended to prevent pryingactionatprestressinggrips. An analytical model was presentedtocalculatetheshearand normal stresses affecting the adhesive layer in the contact area between the CFRP laminate and the steel beam flange. The results of the analytical model were compared to those obtained from finite element analysis, and the accuracy of the calculations along the mid-span was found to be moderately satisfactory. Finally, it was observed that increasing the prestressing force up to 40% enhanced the load capacity and bond strength of the steel-CFRP hybrid section, while higher prestressing levels led to premature rupture failure of the CFRP laminate, significantly reducing the section capacity. The optimum prestressing level was found to be 40% of the CFRP tensile capacity. REFERENCES [1] Young-Chan Youa, Ki-Sun Choia, and JunHee Kim, 2012. An experimental investigationonflexural behaviorofRC beams strengthened with prestressed CFRPstripsusing a durable anchorage system, Composites Part B, ELSEVIER, 2012; 43:3026-3036. [2] Miller, T. C., 2000. The rehabilitation of steel bridge girders using advanced composite materials.” MSc. Thesis. University of Delaware, Newark,Delaware.USA. [3] Miller, T.C., Chajes, M.J., Mertz, D.R., and Hastings, J., 2001. Strengthening of a steel bridge girder using CFRP plates. Journal of Bridge Engineering, ASCE, Vol.6,No.6, pp. 514-522. [4] Young-Chan Y. A., Choi A. K., and Kim J. A., “An experimental investigation on flexural behavior of RC beams strengthened with prestressed CFRPstripsusing a durable anchor-age system”. Composites. Part B, Engineering, ELSEVIER. 2012; 43: 3026-3036. [5] Elawadi A., Orton S. L., Gopalaratnam V., HoltJ.,LopezM. D. Accuracy Evaluation of Pre-stressed Concrete Girder Camber in Missouri Bridges. Journal of Bridge Engineering. Vol. 27, Issue 12 pp 04022119 (December 2022). [6] Ghareeb, M.A, Khadr, M.A., Sayed-Ahmed, E.Y. CFRP Strengthening of Steel I-Beam against Local Web Buckling: A Numerical Analysis. Research and Applications in Structural Engineering, Mechanics & Computation: Proceedings of the Fifth International Conference on Structural Engineering, Mechanics & Computation, A. Zingoni (ed.), Taylor & Francis Group Ltd, Cape Town, South Africa, 2-4 Sept. 2013. [7] M.H. Seleem, I.A. Sharaky, H.E.M. Sallam. Flexural behavior of steel beams strengthened by carbon ﬁber reinforced polymer plates – Three dimensional ﬁnite element simulation. Journal of Materials and Design, ELSEVIER. 2010; 31:1317-1324. [8] Abdelrazik, A, Strengthening of steel I section Beam- Column using Prestressed CFRP Laminates,MSc.Thesis, Ain Shams University Faculty of Engineering, 2013, 154p. [9] Youssef M. “Analytical prediction of the linear and nonlinear behavior of steel beams re-habilitated using FRP sheets”. Journal of Engineering Structures, ELSEVIER. 2006; 28:903-911. [10] Benachour A, Benyoucef S, Tounsi A, Adda bedia E. Inter-facial stress analysis of steel beams reinforced with bonded prestressed FRP plate. Journal of Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072
- 11. International Research Journal of Engineering and Technology (IRJET) e-ISSN: 2395-0056 © 2023, IRJET | Impact Factor value: 8.226 | ISO 9001:2008 Certified Journal | Page 695 Engineering Structures, ELSEVIER. 2008; 30:3305- 3315. [11] Zhao G, Li Alex. Numerical study of a bonded steel and concrete composite beam. ComputerStructure2008;86 (19–20) :1830–8 [12] Sayed-Ahmed, E.Y. 2004. Strengthening of Thin-Walled Steel I-Section Beams Using CFRP Strips. Proceedings, 4th International Conference on Advanced Composite Materials in BridgesandStructures(ACMBSIV),Calgary, Alberta, Canada – CD Proceedings. [13] D. Linghoff, M. Al-Emrani and R. Kliger, (2010) " Performance of steel beams strengthened with CFRP laminate – Part 1: laboratory tests" Composites Part B: Engineering, Vol. 41, No.7, p 509-515. [14] D. Linghoff, M. Al-Emrani and R. Kliger, (2010) " Performance of steel beams strengthened with CFRP laminate – Part 2: FE analyses" Composites Part B: Engineering, Vol. 41, No.7, p 516-522. [15] Al-Emrani M, Kliger R. Analysis of interfacial shear stresses in beams strengthened with bonded prestressed laminates. Journal of Composites Part B: Engineering, ELSEVIER. 2006; 37:265-272. [16] Smith S., Teng J., (2001) “Interfacial stresses in plated beams”. Journal of Engineering Structures, ELSEVIER. 2001; 23: 857-871. [17] SAS, “ANSYS 10 Finite Element Analysis System”, SASIP, Inc 2004 [18] Sayed-Ahmed, E.Y. 2006. Numerical Investigation into Strengthening Steel I-Section Beams Using CFRP Strips. Proceedings, 2006 Structures Congress, ASCE, St. Louis, USA, 18-20 May 2006. [19] Zhaoa, X., Zhang, L., (2007), “State-of-the-art review on FRP strengthened steel structures”, Journal of Engineering Structures, ELSEVIER. 29: 1808-1823. [20] Dawood, M., Rizkalla, S., andSumner,E.,(2007),“Fatigue and Overloading Behavior of Steel–Concrete Composite Flexural Members Strengthened with High Modulus CFRP Materials”.Journal ofCompositesforConstruction, Vol. 11, issue 6. [21] Young-Chan Y. A., Choi A. K., and Kim J. A., “An experimental investigation on flexural behavior of RC beams strengthened with prestressed CFRPstripsusing a durable anchor-age system”. Composites. Part B, Engineering, ELSEVIER. 2012; 43: 3026-3036. [22] Youssef M. “Analytical prediction of the linear and nonlinear behaviour of steel beams rehabilitated using FRP sheets”. Journal of Engineering Structures, ELSEVIER. 2006; 28:903-911. [23] Sallam, H.E.M., Saba, A.M., Shaheen, H.H., and Abdel- Raouf, H. “Prevention of peeling failureinplated beams’’ Journal of Advanced Concrete Technology. 2004; 2(3):419-429. [24] Lam, D. and Clark, K.A., 2003. “Strengthening of steel sections using carbon fiber rein-forced polymers laminate,” Proceedings, Advances in Structures: Steel, Concrete, CompositeandAluminumASSCCA’03,Sydney, Australia, pp. 1369-1374. [25] El-Sisi A., Alsharari F., Salim H., Elawadi A., Hassanin A. “Efficient beam element model for analysisofcomposite beam with partial shear connectivity” Journal of Composite Structures. ELSEVIER. 2023; Vol.303,11626 [26] Gharib, M.A., Khedr., M.A.,Sayed-Ahmed,E.Y.“Interfacial Stress of Steel Beams Strengthened with Prestressed CFRP Laminate And Mechanical Anchorage”. Journal Of Al Azhar University EngineeringSector.Vol.11,Issue38, P:227-238. [27] Sika Corporation, “Sika CarboDur® Carbon fiber laminate for structural strengthening,”Identificationno. 332, 2005. [28] Sika Corporation, “Sikadur® 30 High-modulus, high- strength, structural epoxy paste adhesive for use with Sika CarboDur® reinforcement,” Identification no.332- 15, 2008. Volume: 10 Issue: 02 | Feb 2023 www.irjet.net p-ISSN: 2395-0072